CHIRALITY 26:27–32 (2014)
Chiral 3D Open-Framework Material Ni(D-cam)(H2O)2 Used as GC Stationary Phase SHENGMING XIE,1 BANGJIN WANG,1 XINHUAN ZHANG,1 JUNHUI ZHANG,2 MEI ZHANG,2 AND LIMING YUAN1* 1 Department of Chemistry, Yunnan Normal University, Kunming 650500, P.R. China 2 Department of Chemistry, East China Normal University, Shanghai 200241, P.R. China
ABSTRACT Metal-organic frameworks (MOFs) have been explored for analytical applications because of their outstanding properties such as high surface areas, ﬂexibility and speciﬁc structure features, especially for chromatography application in recent years. In this work, a chiral MOF Ni (D-cam)(H2O)2 with unusual integration of molecular chirality, absolute helicity, and 3-D intrinsic chiral net was chosen as stationary phase to prepare Ni(D-cam)(H2O)2-coated open tubular columns for high-resolution gas chromatographic (GC) separation. Two fused-silica open tubular columns with different inner diameters and lengths, including column A (30 m × 250 μm i.d.) and column B (2 m × 75 μm i.d.), were prepared via a dynamic coating method. The chromatographic properties of the two columns were investigated using n-dodecane as the analyte at 120 °C. The number of theoretical plates (plates/m) of the two metal–organic framework (MOF) columns was 1300 and 2750, respectively. The racemates, isomer and linear alkanes mixture were used as analytes for evaluating the separation properties of Ni(D-cam)(H2O)2-coated open tubular columns. The results showed that the columns offered good separations of isomer and linear alkanes mixture, especially racemates. Chirality 26:27–32, 2013. © 2013 Wiley Periodicals, Inc. KEY WORDS: metal–organic frameworks; open tubular columns; stationary phase; gas chromatography; separation INTRODUCTION
Recently, metal-organic frameworks (MOFs) represent a relatively novel class of hybrid inorganic–organic porous crystalline materials, which have received increasing attention because of their fascinating coordination structures and unusual properties, such as uniform structured nanoscale cavities, high surface area, chemical tunability, as well as excellent chemical and thermal stability. The crystal lattice of the MOFs is constructed by coordination bonds between metal ions or clusters and organic building blocks (multidentate organic ligands). Up to now, a large number of MOFs have been synthesized and obtained diverse applications in many ﬁelds including gas storage, catalysis, drug delivery, sensing and separation, which have been covered in some signiﬁcant reviews.1–9 Particularly, a series of MOFs have been explored for analytical applications because of their diverse structures and unusual properties.10 For instance, MOFs have been used as novel multi-functional materials for direct application to in-ﬁeld sampling,11,12 solid-phase extraction (SPE),13–17 solid-phase microextraction (SPME),18–21 high-resolution gas chromatography (GC),19,22–26 high performance liquid chromatography (HPLC)27–32 and capillary electrophoresis (CE).33 Chirality plays important roles in chemistry and biology, and biological evolution is absolutely dependent on the occurrence of chiral recognition and catalysis. Considering the importance of chiral recognition, tremendous research efforts have been invested into the development of chiral recognition materials. Therefore, the design and synthesis of chiral MOFs have attracted great attention because of their potential applications in chiral separation and asymmetric catalysis. The main advantages for chiral MOFs are that their framework structures, chiral pore environment and functionality can be ﬁnely controlled by the choice of metal ions or clusters and chiral ligands. In recent years, a large number of chiral © 2013 Wiley Periodicals, Inc.
MOFs have been synthesized,34–40 and used as seaparation materials and catalysis. To date, there are only a few studies on Chiral MOFs that are used as chiral stationary phases (CSPs) for separation of racemic compounds in liquid chromatography (LC)41–44 and high-resolution gas chromatography (GC).45–47 MOFs with an intrinsically chiral topology such as quartz, srs, and zeolite beta have attracted interest for decades due to their potential applications in chiral recognition. Chiral Nickel(II) complex containing (+)-camphor has been used as the chiral stationary phase in GC, which exhibited excellent chiral recognition ability for racemic alkyl-substituted cyclic ethers.48 Here we report a chiral MOF Ni(D-cam) (H2O)2 with unusual integration of molecular chirality, absolute helicity, and 3-D intrinsic chiral net (Figure 1) as chiral stationary phase for high-resolution gas chromatographic (GC), which was synthesized by using D-(+)-camphoric acid as ligand according to the method of Zhang et al.49 In this work, we fabricated a Ni(D-cam)(H2O)2-coated open tubular column for separation of organic compounds, including racemates, aromatic isomers and linear alkanes. The chiral column has excellent selectivity and also possesses good recognition ability toward these organic compounds, especially chiral compounds. EXPERIMENTAL Materials and Chemicals All chemicals were of at least analytical grade and used without further treatment. D-(+)-camphoric acid (99%) was purchased from Adamas. Ni *Correspondence to: Li-Ming Yuan, Department of Chemistry, Yunnan Normal University, Kunming 650500, P.R. China. E-mail: [email protected]
com Received for publication 21 June 2013; Accepted 18 September 2013 DOI: 10.1002/chir.22260 Published online 8 November 2013 in Wiley Online Library (wileyonlinelibrary.com).
XIE ET AL.
racemate was 1 μg. The n-alkanes were n-C10 to n-C15 mixture by 3 μg injection mass. The α,β-ionone isomer was 500 ng injection mass. Ethanol (HPLC grade) was given from TEDIA.
Instrumention The scanning electron microscopy (SEM) micrographs were recorded on a Philip model XL30ESEMTMP scanning electron microscope at 30.0 kV. The X-ray diffraction (XRD) patterns were recorded with a D/max-3B diffractometer (Rigaku, Japan) using Cu Kα radiation. The thermogravimetric analysis (TGA) experiment was performed on a ZRY1P simultaneous thermal analyzer (Shanghai, P. R. China) from room 1 temperature to 800 °C at a ramp rate of 10 °C min . All GC separations were performed on a Shimadzu GC-2014C (Kyoto, Japan) system with a ﬂame ionization detector (FID), a split injection port, and a capillary control unit. The instrument control and data acquisition were carried out by the N-2000 software (Zhida Information Engineering Co., Ltd., Zhejiang University, P. R. China). Nitrogen (99.999%) was used as the carrier gas. The inlet temperature of gas chromatograph was set to 200 °C, and the temperature of FID was set to 250 °C.
Synthesis of Ni(D-cam)(H2O)2
Fig. 1. (a) A view of 1-D left-handed M-helix (dashed blue line) in MOF Ni (D-cam)(H2O)2;(b)3-D framework in MOF Ni(D-cam)(H2O)2.
(NO3)6H2O (98%) was purchased from Alfa Aesar. Na2CO3 was from Tianjin Fengchuan Chemical Reagent Science and Technology Co. Ltd. (Tianjin, China). Racemates of citronellal, alanine, methionine, leucine, proline, 1-phenyl-1,2-ethandiol, 2-amino-1-butanol, glutamic acid and phenyl-succinic acid were obtained from Sigma, their injection mass of each
Ni(D-cam)(H2O)2 crystals were synthesized according to Zhang et al.41 Typically, D-camphoric acid (0.1021 g), Na2CO3(0.0503 g), and Ni(NO3) 6H2O (0.3098 g) were dissolved in 7 mL ultrapure water in a 25 mL Teﬂon cup under stirring for 20 min at room temperature. The vessel was then sealed and heated at 120 °C for 5 days. The autoclave was subsequently allowed to cool to room temperature. The green crystals were obtained. Samples for XRD and TGA were dried at 120 °C.
Fabrication of the Ni(D-cam)(H2O)2-coated Open Tubular Column Untreated fused silica capillary columns with a polyimide outer coating were manufactured by Yongnian Optical Fiber Factory (Hebei province, P. R. China). The fused silica open tubular column was treated according to the following method before dynamic coating: the open tubular column
Fig. 2. (a) Simulated and Synthesized XRD patterns of Ni(D-cam)(H2O)2; (b) TGA curve of the prepared Ni(D-cam)(H2O)2; (c) SEM images of Ni(D-cam)(H2O)2 deposited on the inner wall of the open tubular column A; (d) SEM images of the cross section of Ni(D-cam)(H2O)2 coating in part of the open tubular column A. Chirality DOI 10.1002/chir
CHIRAL MOF USED AS STATIONARY PHASE IN GC
was ﬁlled with 1 M NaOH, sealed at both ends, and maintained for 2 h. Thereafter, the open tubular column was washed successively with ultrapure water for 1 h, 0.1 M HCl for 2 h, and ultrapure water again until the outﬂow reached neutrality. The column was then purged with nitrogen for 6 h at 120 °C. The Ni(D-cam)(H2O)2-coated open tubular column was fabricated by a dynamic coating method. Brieﬂy, a 2 mL ethanol suspension of the Ni 1 (D-cam)(H2O)2 ( 1 mg mL ) was introduced into the open tubular column under gas pressure, and then pushed through the column at a rate of 50 cm 1 min to leave a wet coating layer on the inner wall of the open tubular column. A 2 m long buffer tube was attached to the end of the open tubular column as a restrictor to avoid acceleration of the solution plug near the end of the column. Finally, the coated open tubular column was ﬂushed for 6 h with nitrogen and then conditioned from 30 to 250 °C, increasing its temper1 ature at a rate of 1 °C min and was held at 250 °C for 6 h.
RESULTS AND DISCUSSION Characterization of the Synthesized Ni(D-cam)(H2O)2 and Ni(D-cam)(H2O)2-coated Open Tubular Columns
In this study, two Ni(D-cam)(H2O)2-coated open tubular columns with different inner diameters and lengths, including column A (30 m × 250 μm i.d.) and column B (2 m × 75 μm i.d.), were prepared by a dynamic coating method using Ni (D-cam)(H2O)2 as the stationary phase. The column efﬁciency of the two Ni(D-cam)(H2O)2-coated open tubular columns was measured by using n-dodecane as the test compound at 120 °C. The number of theoretical plates (plates/m) of column A and column B were 1300 and 2750, respectively. The prepared Ni(D-cam)(H2O)2 crystals were dried at 120 °C under reduced pressure for XRD characterization. The successful synthesis of Ni(D-cam)(H2O)2 crystals was conﬁrmed by XRD analysis (Figure 2a). Figure 2b shows that the TGA curve of the Ni(D-cam)(H2O)2 crystals, which is stable up to 250 °C and therefore suitable for GC usage. SEM analysis was used to investigate the coating properties of the MOF crystals on the inner wall of the column. The SEM images showed that the column A had an approximately 2 μm thick Ni(D-cam)(H2O)2 coating on the inner wall (Figure 2c and d). To evaluate the classiﬁcation of novel chromatographic stationary phases, the McReynolds constants were used to describe the polarity of Ni(D-cam)(H2O)2-coated open tubular column by choosing benzene, 1-butanol, 2-pentanone,
1-nitropropane, and pyridine as test solutes. The respective constants of the ﬁve selected test solutes are thought to measure various interactions between the stationary phase and the analytes, including weak dispersion forces, polarizability, hydrogen-bonding ability, dipolar and acidic characters of the stationary phase. Squalane is used as a standard nonpolar stationary phase, then the McReynolds constants of the chiral MOF column were compared to that of squalane. The obtained McReynolds constants of ﬁve reference analytes were 153, 254, 192, 166, 391 for benzene, 1-butanol, 2-pentanone, 1-nitropropane and pyridine on column B at 140 °C, respectively. The average of the ﬁve McReynolds constants was 231, which indicates that the polarity of the Ni (D-cam)(H2O)2 is moderate. The elution sequence of the probes was benzene, nitropropane, 2-pentanone, 1-butanoland pyridine. Figure 3 gives the Van Deemter plot of column B for n-dodecane under 120 °C. The optimal linear velocity value of this open tubular column was 11.5 cm s 1 Gas Chromatographic Separation Properties of Ni(D-cam) (H2O)2-coated Open Tubular Column (column B)
In this work, we chose linear alkanes mixture and position isomer as analytes to investigate the separation ability and
Fig. 4. GC chromatograms on the open tubular column B (a) for the separation of alkanes using a temperature program: 50 °C for 0.5min, 40 °C/min to 180 °C, and 3 μg of injection mass of each alkane; (b) for the separation of ionone isomer at 110 °C, and 500 ng of injection mass of α,β-ionone isomer.
TABLE 1. Separation of racemates on column B Racemates citronellal a alanine a methionine a leucine a proline a glutamic acid b 2-amino-1-butanol b 1-phenyl-1,2-ethandiol c phenyl-succinic acid Fig. 3. Van Deemter plot for n-dodecane on capillary column B(2 m long × 75 μm i.d.)under 120 °C.
Retention factor (k1)
Separation factor (α)
100 100 97 105 100 120 120 135 95
1.21 0.96 1.15 0.46 0.49 1.64 1.13 1.67 1.13
1.14 1.56 1.32 2.42 1.99 1.26 1.15 1.22 1.13
a Triﬂuoroacetyl isopropyl ester derivate; btriﬂuoroacetyl derivate; cisopropyl ester derivate.
Chirality DOI 10.1002/chir
XIE ET AL.
Fig. 5. GC chromatograms on the MOF-coated open tubular column B(2 m long × 75 μm i.d.)for the separation of racemates. a) citronellal at 100 °C under a N2 -1 -1 linear velocity of 11.9 cm s ; b) alanine derivative at 100 °C under a N2 linear velocity of 12.5 cm s ; c)methionine derivative at 97 °C under a N2 linear velocity of 12.3 -1 -1 -1 cm s ; d) leucine derivative at 105 °C under a N2 linear velocity of 13.0 cm s ; e) proline derivative at 100 °C under a N2 linear velocity of 13.2 cm s ; f ) glutamic acid -1 -1 derivative at 120 °C under a N2 linear velocity of 11.0 cm s ; g)1-phenyl-1,2-ethandiol derivative at 120 °C under a N2 linear velocity of 11.5 cm s ; h) 2-amino-1-butanol -1 -1 derivative at 135 °C under a N2 linear velocity of 10.0 cm s ; i) phenyl-succinic acid derivative at 95 °C under a N2 linear velocity of 12.1 cm s . 1 μg of injection mass of a b c each racemate. Triﬂuoroacetyl isopropyl ester derivate; triﬂuoroacetyl derivate; isopropyl ester derivate.
selectivity of Ni(D-cam)(H2O)2-coated column. Figure 4a shows that all the seven n-alkanes (n-C10 to n-C16) were baseline separated on the column B with sharp peaks and in a short time by temperature-programmed control. The elution sequence of the seven n-alkanes on the column B follows the order of boiling points because longer linear alkane has stronger Van der Waal’s force with MOF.24 Except for the normal alkanes mixture, the column can separate isomer, and the separation chromatogram of α,β- ionone is shown in Figure 4b. As can be seen from Figure 4b, the α,β- ionone obtained baseline separation on column B. The experimental results show that the Ni(D-cam)(H2O)2 possesses high selectivity and excellent separation performance for alkanes mixture and isomers. In Ni(D-cam)(H2O)2, the enantiopure ligand D-cam coexist with the 3-D intrinsically chiral topology net. In addition, the MOF Ni(D-cam)(H2O)2 has three homochiral features: a 3-D intrinsically homochiral net, homohelicity, and enantiopure molecular chirality. 3-D framework materials with integrated homochiral features have the potential for enhanced chiral recognition and enantioselectivity. Therefore, the chiral 3-D framework Ni(D-cam)(H2O)2 was mainly used for the separation of racemates. Nine racemates were separated on column B, including citronellal, alanine, methionine, leucine, proline, glutamic acid, 2-amino-1-butanol, 1-phenyl-1,2-ethandiol and phenyl-succinic acid. Table 1 showed the retention factors (k1) for the ﬁrst eluted enantiomer and separation factors (α). Their enantiomeric resolutions on column B are exhibited in Figure 5. As can be seen from the separation chromatograms, the column B gave high resolution with short retention times for the enantioseparation of nine racemates, which show baseline separation for all enantiomer pairs except for proline, 1-phenyl-1,2-ethandiol and 2-amino-1-butanol. There are the same elution orders for ﬁve amino acid derivates, in which L enantiomers are eluted after D. Chirality DOI 10.1002/chir
Ni(D-cam)(H2O)2-coated column has excellent chiral recognition ability and selectivity toward racemates due to the inﬂuence of the chiral microenviroment of Ni(D-cam)(H2O)2 with its unusual integration of molecular chirality, left-handed M-helix, and 3-D intrinsic chiral net. Consequently, the chiral recognition ability of the Ni(D-cam)(H2O)2-coated column for the separation of racemates primarily arises from the surface of the crystals in which the steric ﬁt between the homochiral framework and conformation of the solute molecule is the main interactive force.50 Except for these interactions, many other interactions between racemates and chiral MOF Ni(D-cam)(H2O)2 have also enhanced the chiral recognition and enantioselectivity in GC, including hydrogen bonding, dipole-dipole, dispersion, and van der Waals forces. In addition, Ni(D-cam)(H2O)2-coated column (column B) possesses good stability, which can withstand over 500 injections without signiﬁcant decline of selectivity and separation ability under 250 °C.
In conclusion, we have demonstrated a homochiral MOF Ni(D-cam)(H2O)2 as a promising chiral stationary phase for GC separation. The Ni(D-cam)(H2O)2-coated open tubular column showed excellent selectivity. The results presented that chiral MOF Ni(D-cam)(H2O)2 has excellent recognition ability toward alkanes and isomer, especially for racemates.
This work was supported by the National Science Foundation (No. 21275126, No. 21127013).
CHIRAL MOF USED AS STATIONARY PHASE IN GC
LITERATURE CITED 1. Lee JY, Farha OK, Roberts J, Scheidt KA, Nguyen SBT, Hupp JT. Metal-organic framework materials as catalysts. Chem Soc Rev 2009;38:1450–1459. 2. Li JR, Kuppler RJ, Zhou HC. Selective gas adsorption and separation in metal-organic frameworks. Chem Soc Rev 2009;38:1477–1504. 3. Shimomura S, Bureekaew S, Kitagawa S. Porous coordination polymers towards gas technology. Struct Bond 2009;132:51–86. 4. Kurmoo M Magnetic metal–organic frameworks. Chem Soc Rev 2009;38:1353–1379. 5. Kuppler RJ, Timmons DJ, Fang QR, Li JR, Makal TA, Young MD, Yuan DQ, Zhao D, Zhuang WJ, Zhou HC. Potential applications of metal-organic frameworks. Coord Chem Rev 2009;253:3042–3066. 6. Farrusseng D, Aguado S, Pinel C. Metal-organic frameworks: opportunities for catalysis. Angew Chem Int Ed 2009;48:7502–7513. 7. Meek ST, Greathouse JA, Allendorf MD. Metal-Organic Frameworks: A rapidly growing class of versatile nanoporous materials. Adv Mater 2011;23:249–267. 8. Corma A, García H, Llabrés i Xamena FX. Engineering metal organic frameworks for heterogeneous catalysis. Chem Rev 2010;110:4606–4655. 9. Cychosz KA, Ahmad R, Matzger AJ. Liquid phase separations by crystalline microporous coordination polymers. Chem Sci 2010;1:293–302. 10. Gu ZY, Yang CX, Chang N, Yan XP. Metal-organic frameworks for analytical chemistry: from sample collection to chromatographic separation. Acc Chem Res 2012;45:734–745. 11. Ni Z, Jerrell JP, Cadwallader KR, Masel RI. Metal-organic frameworks as adsorbents for trapping and preconcentration of organic phosphonates. Anal Chem 2007;79:1290–1293. 12. Gu, ZY, Wang, G, Yan, XP. MOF-5 metal-organic framework as sorbent for in-ﬁeld sampling and preconcentration in combination with thermal desorption GC/MS for determination of atmospheric formaldehyde. Anal Chem 2010;82:1365–1370. 13. Zhou YY, Yan XP, Kim KN, Wang SW, Liu MG. Exploration of coordination polymer as sorbent for ﬂow injection solid-phase extraction on-line coupled with high-performance liquid chromatography for determination of polycyclic aromatic hydrocarbons in environmental materials. J Chromatogr A 2006;1116:172–178. 14. V de Carvalho PH, Santos Barreto A, Rodrigues MO, de Menezes Prata V, Barreto Alves P, de Mesquita ME, Alves Júnior S, Navickiene S. Twodimensional coordination polymer matrix for solid-phase extraction of pesticide residues from plant Cordia salicifolia. J Sep Sci 2009;32:2132–2138. 15. Barreto AS, da Silva RL, dos Santos Silva SCG, Rodrigues MO, de Simone CA, de Sá GF, Júnior SA, Navickiene S, de Mesquita ME. Potential of a metal-organic framework as a new material for solid-phase extraction of pesticides from lettuce (Lactuca sativa), with analysis by gas chromatography–mass spectrometry. J Sep Sci 2010;33:3811–3816. 16. Gu ZY, Chen YJ, Jiang JQ, Yan XP. Metal-organic frameworks for efﬁcient enrichment of peptides with simultaneous exclusion of proteins from complex biological samples. Chem Commun 2011;47:4787–4789. 17. Ge D, Lee HK. Water stability of zeolite imidazolate framework 8 and application to porous membrane-protected micro-solid-phase extraction of polycyclic aromatic hydrocarbons from environmental water samples. J Chromatogr A 2011;1218:8490–8495. 18. Cui XY, Gu ZY, Jiang DQ, Li Y, Wang HF, Yan XP. In situ hydrothermal growth of metal-organic framework 199 ﬁlms on stainless steel ﬁbers for solid-phase microextraction of gaseous benzene homologues. Anal Chem 2009;81:9771–9777. 19. Chang N, Gu ZY, Wang HF, Yan XP. Metal-organic-framework-based tandem molecular sieves as a dual platform for selective microextraction and high-resolution gas chromatographic separation of n-alkanes in complex matrixes. Anal Chem 2011;83: 7094–7101. 20. Chen XF, Zang H, Wang X, Cheng JG, Zhao RS, Cheng CG, Lu XQ. Metalorganic framework MIL-53(Al) as a solid-phase microextraction adsorbent for the determination of 16 polycyclic aromatic hydrocarbons in water samples by gas chromatography–tandem mass spectrometry. Analyst 2012;137:5411–5419. 21. Yu LQ, Yan XP. Covalent bonding of zeolitic imidazolate framework-90 to functionalized silica ﬁbers for solid-phase microextraction. Chem Commun 2013;49:2142–2144. 22. Gu ZY, Yan XP. Metal-organic framework MIL-101 for high-resolution gaschromatographic separation of xylene isomers and ethylbenzene. Angew Chem Int Ed 2010;49:1477–1480.
23. Chang N, Gu ZY, Yan XP. Zeolitic imidazolate framework-8 nanocrystal coated capillary for molecular sieving of branched alkanes from linear alkanes along with high-resolution chromatographic separation of linear alkanes. J Am Chem Soc 2010;132:13645–13647. 24. Chang N, Yan XP. Exploring reverse shape selectivity and molecular sieving effect of metal-organic framework UIO-66 coated capillary column for gas chromatographic separation. J Chromatogr A 2012;1257:116–124. 25. Gu ZY, Jiang JQ, Yan XP. Fabrication of isoreticular metal-organic framework coated capillary columns for high-resolution gas chromatographic separation of persistent organic pollutants. Anal Chem 2011;83:5093–5100. 26. Fan L, Yan XP. Evaluation of isostructural metal-organic frameworks coated capillary columns for the gas chromatographic separation of alkane isomers. Talanta 2012;99:944–950. 27. Yang CX, Yan XP. Metal-organic framework MIL-101(Cr) for highperformance liquid chromatographic separation of substituted aromatics. Anal Chem 2011;83:7144–7150. 28. Yang CX, Chen YJ, Wang HF, Yan XP. High-performance separation of fullerenes on metal-organic framework MIL-101(Cr). Chem Eur J 2011;17:11734–11737. 29. Fu YY, Yang CX, Yan XP. Control of the coordination status of the open metal sites in metal-organic frameworks for high performance separation of polar compounds. Langmuir 2012;28:6794–6802. 30. Yang CX, Liu SS, Wang HF, Wang SW, Yan XP. High-performance liquid chromatographic separation of position isomers using metal–organic framework MIL-53(Al) as the stationary phase. Analyst 2012;137:133–139. 31. Liu SS, Yang CX, Wang SW, Yan XP. Metal-organic frameworks for reverse-phase high-performance liquid chromatography. Analyst 2012;137:816–818. 32. Fu YY, Yang CX, Yan XP. Metal-organic framework MIL-100(Fe) as the stationary phase for both normal-phase and reverse-phase high performance liquid chromatography. J Chromatogr A 2013;1274:137–144. 33. Li LM, Wang HF, Yan XP. Metal-organic framework ZIF-8 nanocrystals as pseudostationary phase for capillary electrokinetic chromatography. Electrophoresis 2012;33:2896–2902. 34. Zhang J, Liu R, Feng PY, Bu XH. Organic cation and chiral-anion templated 3-D homochiral open-framework materials with unusual square planar M4(OH) units. Angew Chem Int Ed 2007; 46:8388–8391. 35. Zhang J, Chen SM, Valle H, Wong M, Austria C, Cruz M, Bu XH. Manganese and magnesium homochiral materials: decoration of honeycomb channels with homochiral chains. J Am Chem Soc 2007;129:14168–14169. 36. Zhang J, Yao YG, Bu XH. Comparative study of homochiral and racemic chiral metal-organic frameworks built from camphoric acid. Chem Mater 2007;19:5083–5089. 37. Zhang J, Chen SM, Wu T, Feng PY, Bu XH. Homochiral crystallization of microporous framework from achiral precursors by chirality catalysis. J Am Chem Soc 2008;130:12882–12883. 38. Morris RE, Bu XH. Induction of chiral porous solids containing only achiral building blocks. Nat Chem 2010;2:353–361. 39. Zhang J, Chen SM, Nieto RA, Wu T, Feng PY, Bu XH. A tale of three carboxylates: cooperative asymmetric crystallization of 3-D microporous framework from achiral precursors. Angew Chem Int Ed 2010;49:1267–1270. 40. Kang Y, Chen SM, Wang F, Zhang J, Bu XH. Induction in urothermal synthesis of chiral porous materials from achiral precursors. Chem Commun 2011;47:4950–4952. 41. Nuzhdin AL, Dybtsev DN, Bryliakov KP, Talsi EP, Fedin VP. Enantioselective chromatographic resolution and one-pot synthesis of enantiomerically pure sulfoxides over a homochiral Zn-organic framework. J Am Chem Soc 2007; 129:12958–12959. 42. Padmanaban M, Müller P, Lieder C, Gedrich K, Grünker R, Bon V, Senkovska I, Baumgärtner S, Opelt S, Paasch S, Brunner E, Glorius F, Klemm E, Kaskel S. Application of a chiral metal-organic framework in enantioselective separation. Chem Commun 2011;47:12089–12091. 43. Tanaka K, Muraoka T, Hirayama D, Ohnish A. Highly efﬁcient chromatographic resolution of sulfoxides using a new homochiral MOF-silica composite. Chem Commun 2012;48:8577–8579. 44. Zhang M, Pu ZJ, Chen XL, Gong XL, Zhu AX, Yuan LM. Chiral recognition of a 3D chiral nanoporous metal-organic framework. Chem Commun 2013;49:5201–5203. 45. Xie SM, Zhang ZJ, Wang ZY, Yuan LM. Chiral metal-organic frameworks for high-resolution gas chromatographic separations. J Am Chem Soc 2011;133:11892–11895. Chirality DOI 10.1002/chir
XIE ET AL.
46. Xie SM, Zhang XH, Zhang ZJ, Yuan LM. Porous chiral metal-organic framework InH(D-C10H14O4)2 with anionic-type diamond network for high-resolution gas chromatographic enantioseparations. Anal Lett 2013;46:753–763. 47. Xie SM, Zhang XH, Zhang ZJ, Zhang M, Jia J, Yuan LM. A 3-D open-framework material with intrinsic chiral topology used as a stationary phase in gas chromatography. Anal Bioanal Chem 2013;405:3407–3412.
Chirality DOI 10.1002/chir
48. Schurig V, Bürkle W. Extending the scope of enantiomer resolution by complexation gas chromatography. J Am Chem Soc 1982;104:7573–7580. 49. Zhang J, Chen SM, Zingiryan A, Bu XH. Integrated molecular chirality, absolute helicity, and intrinsic chiral topology in three-dimensional open-framework materials. J Am Chem Soc 2008;130:17246–17247. 50. Ikai T, Okamoto Y. Structure control of polysaccharide derivatives for efﬁcient separation of enantiomers by chromatography. Chem Rev 2009;109:6077–6101.